Strong Second Harmonic Generation in a Tungsten Bronze Oxide by Enhancing Local Structural Distortion.
Lin, Kun; Gong, Pifu; Chu, Shihang; Li, Qiang; Lin, Zheshuai; Wu, Hui; Wang, Qingxiao; Wang, Jinguo; Kim, Moon J.; Kato, Kenichi; Wang, Chin-Wei; Liu, Xinzhi; Huang, Qingzhen; Chen, Jun; Zhu, He; Deng, Jinxia; Xing, Xianran; Journal of the American Chemical Society 142 (2020) 7480–7486; doi:10.1021/jacs.0c00133

data_4134711
_publ_section_title
;
 Strong Second Harmonic Generation in a Tungsten Bronze Oxide by Enhancing
 Local Structural Distortion.
;
_journal_issue                   16
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7480
_journal_page_last               7486
_journal_paper_doi               10.1021/jacs.0c00133
_journal_volume                  142
_journal_year                    2020
_chemical_formula_sum            'Li0.687 Nb5 O15 Pb2.157'
_chemical_formula_weight         1156.2
_space_group_IT_number           31
_space_group_name_Hall           'P -2 -2bc'
_space_group_name_H-M_alt        'P n 21 m'
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      31
_symmetry_space_group_name_Hall  'P -2 -2bc'
_symmetry_space_group_name_H-M   'P n 21 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.38233(11)
_cell_length_b                   12.66874(12)
_cell_length_c                   7.66215(6)
_cell_measurement_temperature    300
_cell_volume                     1201.950(18)
_diffrn_ambient_temperature      300
_diffrn_measurement_device       BT-1
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     2.0775
_exptl_absorpt_coefficient_mu    0.021
_exptl_crystal_density_diffrn    6.3893
_exptl_crystal_F_000             2016
_pd_char_colour                  colourless
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        166.450
_pd_meas_2theta_range_min        3.000
_pd_meas_number_of_points        3270
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        166.45
_pd_proc_2theta_range_min        3
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.0123
_pd_proc_ls_prof_wR_expected     0.0301
_pd_proc_ls_prof_wR_factor       0.0195
_refine_diff_density_max         0.19
_refine_diff_density_min         -0.22
_refine_ls_goodness_of_fit_all   2.13
_refine_ls_number_constraints    2
_refine_ls_number_parameters     157
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0880
_refine_ls_R_factor_gt           0.0787
_refine_ls_shift/su_max          0.0000
_refine_ls_shift/su_mean         0.0000
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_all         0.0653
_refine_ls_wR_factor_gt          0.0629
_cod_data_source_file            ja0c00133_si_002.cif
_cod_data_source_block           I
_cod_depositor_comments          'Adding full bibliography for 4134711.cif.'
_cod_original_sg_symbol_Hall     'P -2xbc;2ybc;-2z'
_cod_database_code               4134711
_publcif_funding_html
;
;